# Electronic Supplementary Material (ESI) for Journal of Materials Chemistry C.
# This journal is © The Royal Society of Chemistry 2019

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_K2NaGaF6
_audit_block_doi                 10.25505/fiz.icsd.cc223p30
_database_code_depnum_ccdc_archive 'CCDC 1910161'
_audit_update_record             
;
2019-04-15 deposited with the CCDC.	2019-06-03 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2016/6
_shelx_SHELXL_version_number     2016/6
_chemical_name_systematic        ?
_chemical_name_common            K2NaGaF6
_chemical_melting_point          ?
_chemical_formula_moiety         'F12 Ga2 K4 Na2'
_chemical_formula_sum            'F12 Ga2 K4 Na2'
_chemical_formula_weight         569.82

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.2307 1.6083 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      cubic
_space_group_IT_number           225
_space_group_name_H-M_alt        'F m -3 m'
_space_group_name_Hall           '-F 4 2 3'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'z, x, y'
'z, -x, -y'
'-z, -x, y'
'-z, x, -y'
'y, z, x'
'-y, z, -x'
'y, -z, -x'
'-y, -z, x'
'y, x, -z'
'-y, -x, -z'
'y, -x, z'
'-y, x, z'
'x, z, -y'
'-x, z, y'
'-x, -z, -y'
'x, -z, y'
'z, y, -x'
'z, -y, x'
'-z, y, x'
'-z, -y, -x'
'x, y+1/2, z+1/2'
'-x, -y+1/2, z+1/2'
'-x, y+1/2, -z+1/2'
'x, -y+1/2, -z+1/2'
'z, x+1/2, y+1/2'
'z, -x+1/2, -y+1/2'
'-z, -x+1/2, y+1/2'
'-z, x+1/2, -y+1/2'
'y, z+1/2, x+1/2'
'-y, z+1/2, -x+1/2'
'y, -z+1/2, -x+1/2'
'-y, -z+1/2, x+1/2'
'y, x+1/2, -z+1/2'
'-y, -x+1/2, -z+1/2'
'y, -x+1/2, z+1/2'
'-y, x+1/2, z+1/2'
'x, z+1/2, -y+1/2'
'-x, z+1/2, y+1/2'
'-x, -z+1/2, -y+1/2'
'x, -z+1/2, y+1/2'
'z, y+1/2, -x+1/2'
'z, -y+1/2, x+1/2'
'-z, y+1/2, x+1/2'
'-z, -y+1/2, -x+1/2'
'x+1/2, y, z+1/2'
'-x+1/2, -y, z+1/2'
'-x+1/2, y, -z+1/2'
'x+1/2, -y, -z+1/2'
'z+1/2, x, y+1/2'
'z+1/2, -x, -y+1/2'
'-z+1/2, -x, y+1/2'
'-z+1/2, x, -y+1/2'
'y+1/2, z, x+1/2'
'-y+1/2, z, -x+1/2'
'y+1/2, -z, -x+1/2'
'-y+1/2, -z, x+1/2'
'y+1/2, x, -z+1/2'
'-y+1/2, -x, -z+1/2'
'y+1/2, -x, z+1/2'
'-y+1/2, x, z+1/2'
'x+1/2, z, -y+1/2'
'-x+1/2, z, y+1/2'
'-x+1/2, -z, -y+1/2'
'x+1/2, -z, y+1/2'
'z+1/2, y, -x+1/2'
'z+1/2, -y, x+1/2'
'-z+1/2, y, x+1/2'
'-z+1/2, -y, -x+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, -z'
'z+1/2, x+1/2, y'
'z+1/2, -x+1/2, -y'
'-z+1/2, -x+1/2, y'
'-z+1/2, x+1/2, -y'
'y+1/2, z+1/2, x'
'-y+1/2, z+1/2, -x'
'y+1/2, -z+1/2, -x'
'-y+1/2, -z+1/2, x'
'y+1/2, x+1/2, -z'
'-y+1/2, -x+1/2, -z'
'y+1/2, -x+1/2, z'
'-y+1/2, x+1/2, z'
'x+1/2, z+1/2, -y'
'-x+1/2, z+1/2, y'
'-x+1/2, -z+1/2, -y'
'x+1/2, -z+1/2, y'
'z+1/2, y+1/2, -x'
'z+1/2, -y+1/2, x'
'-z+1/2, y+1/2, x'
'-z+1/2, -y+1/2, -x'
'-x, -y, -z'
'x, y, -z'
'x, -y, z'
'-x, y, z'
'-z, -x, -y'
'-z, x, y'
'z, x, -y'
'z, -x, y'
'-y, -z, -x'
'y, -z, x'
'-y, z, x'
'y, z, -x'
'-y, -x, z'
'y, x, z'
'-y, x, -z'
'y, -x, -z'
'-x, -z, y'
'x, -z, -y'
'x, z, y'
'-x, z, -y'
'-z, -y, x'
'-z, y, -x'
'z, -y, -x'
'z, y, x'
'-x, -y+1/2, -z+1/2'
'x, y+1/2, -z+1/2'
'x, -y+1/2, z+1/2'
'-x, y+1/2, z+1/2'
'-z, -x+1/2, -y+1/2'
'-z, x+1/2, y+1/2'
'z, x+1/2, -y+1/2'
'z, -x+1/2, y+1/2'
'-y, -z+1/2, -x+1/2'
'y, -z+1/2, x+1/2'
'-y, z+1/2, x+1/2'
'y, z+1/2, -x+1/2'
'-y, -x+1/2, z+1/2'
'y, x+1/2, z+1/2'
'-y, x+1/2, -z+1/2'
'y, -x+1/2, -z+1/2'
'-x, -z+1/2, y+1/2'
'x, -z+1/2, -y+1/2'
'x, z+1/2, y+1/2'
'-x, z+1/2, -y+1/2'
'-z, -y+1/2, x+1/2'
'-z, y+1/2, -x+1/2'
'z, -y+1/2, -x+1/2'
'z, y+1/2, x+1/2'
'-x+1/2, -y, -z+1/2'
'x+1/2, y, -z+1/2'
'x+1/2, -y, z+1/2'
'-x+1/2, y, z+1/2'
'-z+1/2, -x, -y+1/2'
'-z+1/2, x, y+1/2'
'z+1/2, x, -y+1/2'
'z+1/2, -x, y+1/2'
'-y+1/2, -z, -x+1/2'
'y+1/2, -z, x+1/2'
'-y+1/2, z, x+1/2'
'y+1/2, z, -x+1/2'
'-y+1/2, -x, z+1/2'
'y+1/2, x, z+1/2'
'-y+1/2, x, -z+1/2'
'y+1/2, -x, -z+1/2'
'-x+1/2, -z, y+1/2'
'x+1/2, -z, -y+1/2'
'x+1/2, z, y+1/2'
'-x+1/2, z, -y+1/2'
'-z+1/2, -y, x+1/2'
'-z+1/2, y, -x+1/2'
'z+1/2, -y, -x+1/2'
'z+1/2, y, x+1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, z'
'-z+1/2, -x+1/2, -y'
'-z+1/2, x+1/2, y'
'z+1/2, x+1/2, -y'
'z+1/2, -x+1/2, y'
'-y+1/2, -z+1/2, -x'
'y+1/2, -z+1/2, x'
'-y+1/2, z+1/2, x'
'y+1/2, z+1/2, -x'
'-y+1/2, -x+1/2, z'
'y+1/2, x+1/2, z'
'-y+1/2, x+1/2, -z'
'y+1/2, -x+1/2, -z'
'-x+1/2, -z+1/2, y'
'x+1/2, -z+1/2, -y'
'x+1/2, z+1/2, y'
'-x+1/2, z+1/2, -y'
'-z+1/2, -y+1/2, x'
'-z+1/2, y+1/2, -x'
'z+1/2, -y+1/2, -x'
'z+1/2, y+1/2, x'

_cell_length_a                   8.2101(3)
_cell_length_b                   8.2101(3)
_cell_length_c                   8.2101(3)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     553.41(6)
_cell_formula_units_Z            2
_cell_measurement_temperature    100(2)
_cell_measurement_reflns_used    292
_cell_measurement_theta_min      4.30
_cell_measurement_theta_max      26.60

_exptl_crystal_description       block
_exptl_crystal_colour            colourless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    3.420
_exptl_crystal_F_000             536
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.1
_exptl_crystal_size_mid          0.1
_exptl_crystal_size_min          0.1
_exptl_absorpt_coefficient_mu    6.595
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.5947
_exptl_absorpt_correction_T_max  0.7454
_exptl_absorpt_process_details   
'The following wavelength and cell were deduced by SADABS from the direction cosines etc. They are given here for emergency use only: CELL 0.71073    8.213    8.214    8.213   90.000   90.000   90.000'
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      100(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   'fine-focus sealed tube'
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'fine-focus sealed tube'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            447
_diffrn_reflns_av_unetI/netI     0.0174
_diffrn_reflns_av_R_equivalents  0.0322
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_theta_min         4.299
_diffrn_reflns_theta_max         26.732
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.981
_diffrn_measured_fraction_theta_full 0.976
_diffrn_reflns_Laue_measured_fraction_max 0.981
_diffrn_reflns_Laue_measured_fraction_full 0.976
_diffrn_reflns_point_group_measured_fraction_max 0.981
_diffrn_reflns_point_group_measured_fraction_full 0.976
_reflns_number_total             51
_reflns_number_gt                51
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SMART'
_computing_structure_solution    'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_molecular_graphics    'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_publication_material  'Diamond 3.0'
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0406P)²] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         51
_refine_ls_number_parameters     7
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0268
_refine_ls_R_factor_gt           0.0268
_refine_ls_wR_factor_ref         0.0601
_refine_ls_wR_factor_gt          0.0601
_refine_ls_goodness_of_fit_ref   1.279
_refine_ls_restrained_S_all      1.279
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ga1 Ga 0.000000 0.500000 0.500000 0.0021(5) Uani 1 48 d S T P . .
K1 K 0.250000 0.750000 0.750000 0.0074(6) Uani 1 24 d S T P . .
Na1 Na 0.000000 1.000000 0.500000 0.0055(11) Uani 1 48 d S T P . .
F1 F 0.000000 0.7296(3) 0.500000 0.0076(7) Uani 1 8 d S T P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ga1 F1 1.885(3) . ?
Ga1 F1 1.885(3) 57_455 ?
Ga1 F1 1.885(3) 153_565 ?
Ga1 F1 1.885(3) 173_556 ?
Ga1 F1 1.885(3) 77_455 ?
Ga1 F1 1.885(3) 97_566 ?
Ga1 K1 3.55508(13) 97_566 ?
Ga1 K1 3.55508(13) 25_544 ?
Ga1 K1 3.55508(13) 121_566 ?
Ga1 K1 3.55508(13) 145_566 ?
Ga1 K1 3.55508(13) 169_566 ?
Ga1 K1 3.55508(13) 73_445 ?
K1 F1 2.90755(19) 57_455 ?
K1 F1 2.90755(19) 77_455 ?
K1 F1 2.90755(18) 81_456 ?
K1 F1 2.90755(19) 5_565 ?
K1 F1 2.90755(19) 49 ?
K1 F1 2.90755(19) 149_566 ?
K1 F1 2.90755(18) 125_656 ?
K1 F1 2.90755(19) 169_566 ?
K1 F1 2.90755(19) 121_566 ?
K1 F1 2.90755(18) 105_666 ?
K1 F1 2.90755(19) 129_665 ?
K1 Na1 3.55508(13) 49 ?
Na1 F1 2.220(3) 33_455 ?
Na1 F1 2.220(3) 129_665 ?
Na1 F1 2.220(3) 149_566 ?
Na1 F1 2.220(3) 53_464 ?
Na1 F1 2.220(3) 97_576 ?
Na1 F1 2.220(3) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
F1 Ga1 F1 90.000(1) . 57_455 ?
F1 Ga1 F1 90.0 . 153_565 ?
F1 Ga1 F1 180.0 57_455 153_565 ?
F1 Ga1 F1 90.0 . 173_556 ?
F1 Ga1 F1 90.0 57_455 173_556 ?
F1 Ga1 F1 90.0 153_565 173_556 ?
F1 Ga1 F1 90.0 . 77_455 ?
F1 Ga1 F1 90.0 57_455 77_455 ?
F1 Ga1 F1 90.0 153_565 77_455 ?
F1 Ga1 F1 180.0 173_556 77_455 ?
F1 Ga1 F1 180.0 . 97_566 ?
F1 Ga1 F1 90.0 57_455 97_566 ?
F1 Ga1 F1 90.000(1) 153_565 97_566 ?
F1 Ga1 F1 90.0 173_556 97_566 ?
F1 Ga1 F1 90.0 77_455 97_566 ?
F1 Ga1 K1 125.3 . 97_566 ?
F1 Ga1 K1 125.3 57_455 97_566 ?
F1 Ga1 K1 54.7 153_565 97_566 ?
F1 Ga1 K1 54.7 173_556 97_566 ?
F1 Ga1 K1 125.3 77_455 97_566 ?
F1 Ga1 K1 54.7 97_566 97_566 ?
F1 Ga1 K1 125.3 . 25_544 ?
F1 Ga1 K1 54.7 57_455 25_544 ?
F1 Ga1 K1 125.3 153_565 25_544 ?
F1 Ga1 K1 54.7 173_556 25_544 ?
F1 Ga1 K1 125.3 77_455 25_544 ?
F1 Ga1 K1 54.7 97_566 25_544 ?
K1 Ga1 K1 70.5 97_566 25_544 ?
F1 Ga1 K1 54.7 . 121_566 ?
F1 Ga1 K1 125.3 57_455 121_566 ?
F1 Ga1 K1 54.7 153_565 121_566 ?
F1 Ga1 K1 125.3 173_556 121_566 ?
F1 Ga1 K1 54.7 77_455 121_566 ?
F1 Ga1 K1 125.3 97_566 121_566 ?
K1 Ga1 K1 109.5 97_566 121_566 ?
K1 Ga1 K1 180.0 25_544 121_566 ?
F1 Ga1 K1 125.3 . 145_566 ?
F1 Ga1 K1 54.7 57_455 145_566 ?
F1 Ga1 K1 125.3 153_565 145_566 ?
F1 Ga1 K1 125.3 173_556 145_566 ?
F1 Ga1 K1 54.7 77_455 145_566 ?
F1 Ga1 K1 54.7 97_566 145_566 ?
K1 Ga1 K1 109.5 97_566 145_566 ?
K1 Ga1 K1 70.5 25_544 145_566 ?
K1 Ga1 K1 109.5 121_566 145_566 ?
F1 Ga1 K1 54.7 . 169_566 ?
F1 Ga1 K1 54.7 57_455 169_566 ?
F1 Ga1 K1 125.3 153_565 169_566 ?
F1 Ga1 K1 54.7 173_556 169_566 ?
F1 Ga1 K1 125.3 77_455 169_566 ?
F1 Ga1 K1 125.3 97_566 169_566 ?
K1 Ga1 K1 109.5 97_566 169_566 ?
K1 Ga1 K1 70.5 25_544 169_566 ?
K1 Ga1 K1 109.5 121_566 169_566 ?
K1 Ga1 K1 109.5 145_566 169_566 ?
F1 Ga1 K1 125.3 . 73_445 ?
F1 Ga1 K1 125.3 57_455 73_445 ?
F1 Ga1 K1 54.7 153_565 73_445 ?
F1 Ga1 K1 125.3 173_556 73_445 ?
F1 Ga1 K1 54.7 77_455 73_445 ?
F1 Ga1 K1 54.7 97_566 73_445 ?
K1 Ga1 K1 70.5 97_566 73_445 ?
K1 Ga1 K1 109.5 25_544 73_445 ?
K1 Ga1 K1 70.5 121_566 73_445 ?
K1 Ga1 K1 70.5 145_566 73_445 ?
K1 Ga1 K1 180.0 169_566 73_445 ?
F1 K1 F1 54.56(8) 57_455 77_455 ?
F1 K1 F1 173.39(10) 57_455 81_456 ?
F1 K1 F1 119.890(4) 77_455 81_456 ?
F1 K1 F1 119.890(3) 57_455 5_565 ?
F1 K1 F1 173.39(10) 77_455 5_565 ?
F1 K1 F1 65.36(8) 81_456 5_565 ?
F1 K1 F1 119.890(3) 57_455 49 ?
F1 K1 F1 119.890(3) 77_455 49 ?
F1 K1 F1 65.36(8) 81_456 49 ?
F1 K1 F1 65.36(8) 5_565 49 ?
F1 K1 F1 119.890(3) 57_455 149_566 ?
F1 K1 F1 90.191(6) 77_455 149_566 ?
F1 K1 F1 54.56(8) 81_456 149_566 ?
F1 K1 F1 90.191(6) 5_565 149_566 ?
F1 K1 F1 119.890(3) 49 149_566 ?
F1 K1 F1 65.36(8) 57_455 125_656 ?
F1 K1 F1 90.191(6) 77_455 125_656 ?
F1 K1 F1 119.890(3) 81_456 125_656 ?
F1 K1 F1 90.191(6) 5_565 125_656 ?
F1 K1 F1 54.56(8) 49 125_656 ?
F1 K1 F1 173.39(10) 149_566 125_656 ?
F1 K1 F1 65.36(8) 57_455 169_566 ?
F1 K1 F1 119.890(3) 77_455 169_566 ?
F1 K1 F1 119.890(3) 81_456 169_566 ?
F1 K1 F1 54.56(8) 5_565 169_566 ?
F1 K1 F1 90.191(6) 49 169_566 ?
F1 K1 F1 119.890(3) 149_566 169_566 ?
F1 K1 F1 65.36(8) 125_656 169_566 ?
F1 K1 F1 119.890(3) 57_455 121_566 ?
F1 K1 F1 65.36(8) 77_455 121_566 ?
F1 K1 F1 54.56(8) 81_456 121_566 ?
F1 K1 F1 119.890(3) 5_565 121_566 ?
F1 K1 F1 90.191(6) 49 121_566 ?
F1 K1 F1 54.56(8) 149_566 121_566 ?
F1 K1 F1 119.890(3) 125_656 121_566 ?
F1 K1 F1 173.39(10) 169_566 121_566 ?
F1 K1 F1 90.191(6) 57_455 105_666 ?
F1 K1 F1 65.36(8) 77_455 105_666 ?
F1 K1 F1 90.191(6) 81_456 105_666 ?
F1 K1 F1 119.890(4) 5_565 105_666 ?
F1 K1 F1 54.56(8) 49 105_666 ?
F1 K1 F1 119.890(3) 149_566 105_666 ?
F1 K1 F1 54.56(8) 125_656 105_666 ?
F1 K1 F1 119.890(3) 169_566 105_666 ?
F1 K1 F1 65.36(8) 121_566 105_666 ?
F1 K1 F1 90.191(6) 57_455 129_665 ?
F1 K1 F1 119.890(3) 77_455 129_665 ?
F1 K1 F1 90.191(6) 81_456 129_665 ?
F1 K1 F1 54.56(8) 5_565 129_665 ?
F1 K1 F1 119.890(4) 49 129_665 ?
F1 K1 F1 65.36(8) 149_566 129_665 ?
F1 K1 F1 119.890(3) 125_656 129_665 ?
F1 K1 F1 54.56(8) 169_566 129_665 ?
F1 K1 F1 119.890(3) 121_566 129_665 ?
F1 K1 F1 173.39(10) 105_666 129_665 ?
F1 K1 Na1 148.04(5) 57_455 49 ?
F1 K1 Na1 148.04(5) 77_455 49 ?
F1 K1 Na1 38.57(5) 81_456 49 ?
F1 K1 Na1 38.57(5) 5_565 49 ?
F1 K1 Na1 38.57(5) 49 49 ?
F1 K1 Na1 88.09(3) 149_566 49 ?
F1 K1 Na1 88.09(3) 125_656 49 ?
F1 K1 Na1 88.09(3) 169_566 49 ?
F1 K1 Na1 88.09(3) 121_566 49 ?
F1 K1 Na1 88.09(3) 105_666 49 ?
F1 K1 Na1 88.09(3) 129_665 49 ?
F1 Na1 F1 180.0 33_455 129_665 ?
F1 Na1 F1 90.0 33_455 149_566 ?
F1 Na1 F1 90.0 129_665 149_566 ?
F1 Na1 F1 90.0 33_455 53_464 ?
F1 Na1 F1 90.0 129_665 53_464 ?
F1 Na1 F1 180.0 149_566 53_464 ?
F1 Na1 F1 90.0 33_455 97_576 ?
F1 Na1 F1 90.000(1) 129_665 97_576 ?
F1 Na1 F1 90.0 149_566 97_576 ?
F1 Na1 F1 90.0 53_464 97_576 ?
F1 Na1 F1 90.000(1) 33_455 . ?
F1 Na1 F1 90.0 129_665 . ?
F1 Na1 F1 90.0 149_566 . ?
F1 Na1 F1 90.0 53_464 . ?
F1 Na1 F1 180.0 97_576 . ?
F1 Na1 K1 54.7 33_455 49_454 ?
F1 Na1 K1 125.3 129_665 49_454 ?
F1 Na1 K1 125.3 149_566 49_454 ?
F1 Na1 K1 54.7 53_464 49_454 ?
F1 Na1 K1 125.3 97_576 49_454 ?
F1 Na1 K1 54.7 . 49_454 ?
F1 Na1 K1 125.3 33_455 145_576 ?
F1 Na1 K1 54.7 129_665 145_576 ?
F1 Na1 K1 54.7 149_566 145_576 ?
F1 Na1 K1 125.3 53_464 145_576 ?
F1 Na1 K1 54.7 97_576 145_576 ?
F1 Na1 K1 125.3 . 145_576 ?
K1 Na1 K1 180.0 49_454 145_576 ?
F1 Na1 K1 54.7 33_455 73_455 ?
F1 Na1 K1 125.3 129_665 73_455 ?
F1 Na1 K1 54.7 149_566 73_455 ?
F1 Na1 K1 125.3 53_464 73_455 ?
F1 Na1 K1 54.7 97_576 73_455 ?
F1 Na1 K1 125.3 . 73_455 ?
K1 Na1 K1 109.471(1) 49_454 73_455 ?
K1 Na1 K1 70.529(1) 145_576 73_455 ?
F1 Na1 K1 125.3 33_455 169_566 ?
F1 Na1 K1 54.7 129_665 169_566 ?
F1 Na1 K1 125.3 149_566 169_566 ?
F1 Na1 K1 54.7 53_464 169_566 ?
F1 Na1 K1 125.3 97_576 169_566 ?
F1 Na1 K1 54.7 . 169_566 ?
K1 Na1 K1 70.5 49_454 169_566 ?
K1 Na1 K1 109.471(1) 145_576 169_566 ?
K1 Na1 K1 180.0 73_455 169_566 ?
F1 Na1 K1 54.7 33_455 97_576 ?
F1 Na1 K1 125.3 129_665 97_576 ?
F1 Na1 K1 125.3 149_566 97_576 ?
F1 Na1 K1 54.7 53_464 97_576 ?
F1 Na1 K1 54.736(1) 97_576 97_576 ?
F1 Na1 K1 125.264(1) . 97_576 ?
K1 Na1 K1 70.5 49_454 97_576 ?
K1 Na1 K1 109.5 145_576 97_576 ?
K1 Na1 K1 70.5 73_455 97_576 ?
K1 Na1 K1 109.5 169_566 97_576 ?
F1 Na1 K1 54.7 33_455 121_566 ?
F1 Na1 K1 125.3 129_665 121_566 ?
F1 Na1 K1 54.7 149_566 121_566 ?
F1 Na1 K1 125.3 53_464 121_566 ?
F1 Na1 K1 125.3 97_576 121_566 ?
F1 Na1 K1 54.7 . 121_566 ?
K1 Na1 K1 70.529(1) 49_454 121_566 ?
K1 Na1 K1 109.471(1) 145_576 121_566 ?
K1 Na1 K1 70.529(1) 73_455 121_566 ?
K1 Na1 K1 109.5 169_566 121_566 ?
K1 Na1 K1 109.5 97_576 121_566 ?
Ga1 F1 Na1 180.0 . . ?
Ga1 F1 K1 93.31(5) . 49_454 ?
Na1 F1 K1 86.69(5) . 49_454 ?
Ga1 F1 K1 93.31(5) . 121_566 ?
Na1 F1 K1 86.69(5) . 121_566 ?
K1 F1 K1 89.809(6) 49_454 121_566 ?
Ga1 F1 K1 93.31(5) . 169_566 ?
Na1 F1 K1 86.69(5) . 169_566 ?
K1 F1 K1 89.809(6) 49_454 169_566 ?
K1 F1 K1 173.39(10) 121_566 169_566 ?

_refine_diff_density_max         0.555
_refine_diff_density_min         -0.849
_refine_diff_density_rms         0.216

